General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8.4 - 8.5 g/cm³ Show Material materials with Density of 8.4 - 8.5 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 209 GPa Show Material materials with Elastic modulus of 209 GPa |

100.0 °C | 202 GPa Show Material materials with Elastic modulus of 202 GPa | |

200.0 °C | 195 GPa Show Material materials with Elastic modulus of 195 GPa | |

300.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | |

400.0 °C | 185 GPa Show Material materials with Elastic modulus of 185 GPa | |

500.0 °C | 178 GPa Show Material materials with Elastic modulus of 178 GPa | |

600.0 °C | 170 GPa Show Material materials with Elastic modulus of 170 GPa | |

700.0 °C | 162 GPa Show Material materials with Elastic modulus of 162 GPa | |

800.0 °C | 153 GPa Show Material materials with Elastic modulus of 153 GPa | |

900.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | |

1000.0 °C | 128 GPa Show Material materials with Elastic modulus of 128 GPa | |

Elongation | 20.0 °C | 30 - 40 % Show Material materials with Elongation of 30 - 40 % |

Elongation A100 | 20.0 °C | 25 - 35 % Show Material materials with Elongation A100 of 25 - 35 % |

Elongation A80, transverse | 20.0 °C | 30 - 35 % Show Material materials with Elongation A80, transverse of 30 - 35 % |

Elongation, transverse | 20.0 °C | 30 - 35 % Show Material materials with Elongation, transverse of 30 - 35 % |

Hardness, Brinell | 20.0 °C | 240 [-] Show Material materials with Hardness, Brinell of 240 [-] |

Tensile strength | 20.0 °C | 700 - 1000 MPa Show Material materials with Tensile strength of 700 - 1000 MPa |

100.0 °C | 600 - 740 MPa Show Material materials with Tensile strength of 600 - 740 MPa | |

200.0 °C | 580 - 700 MPa Show Material materials with Tensile strength of 580 - 700 MPa | |

300.0 °C | 560 - 685 MPa Show Material materials with Tensile strength of 560 - 685 MPa | |

400.0 °C | 543 - 670 MPa Show Material materials with Tensile strength of 543 - 670 MPa | |

450.0 °C | 530 - 660 MPa Show Material materials with Tensile strength of 530 - 660 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 20.0 °C | 760 - 1000 MPa Show Material materials with Tensile strength, transverse of 760 - 1000 MPa |

Yield strength Rp0.2 | 20.0 °C | 330 - 415 MPa Show Material materials with Yield strength Rp0.2 of 330 - 415 MPa |

100.0 °C | 290 - 350 MPa Show Material materials with Yield strength Rp0.2 of 290 - 350 MPa | |

200.0 °C | 265 - 320 MPa Show Material materials with Yield strength Rp0.2 of 265 - 320 MPa | |

300.0 °C | 260 - 300 MPa Show Material materials with Yield strength Rp0.2 of 260 - 300 MPa | |

400.0 °C | 260 - 280 MPa Show Material materials with Yield strength Rp0.2 of 260 - 280 MPa | |

450.0 °C | 255 - 270 MPa Show Material materials with Yield strength Rp0.2 of 255 - 270 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 380 - 400 MPa Show Material materials with Yield strength Rp0.2, transverse of 380 - 400 MPa |

Yield strength Rp1.0 | 20.0 °C | 375 - 445 MPa Show Material materials with Yield strength Rp1.0 of 375 - 445 MPa |

Thermal

Property | Temperature | Value |
---|---|---|

Coefficient of thermal expansion | 100.0 °C | 1.28E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.28E-5 1/K |

200.0 °C | 1.11E-5 - 1.31E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.11E-5 - 1.31E-5 1/K | |

300.0 °C | 1.34E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.34E-5 1/K | |

400.0 °C | 1.26E-5 - 1.37E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.26E-5 - 1.37E-5 1/K | |

500.0 °C | 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.41E-5 1/K | |

600.0 °C | 1.38E-5 - 1.46E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.38E-5 - 1.46E-5 1/K | |

700.0 °C | 1.52E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.52E-5 1/K | |

800.0 °C | 1.49E-5 - 1.58E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 - 1.58E-5 1/K | |

900.0 °C | 1.64E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.64E-5 1/K | |

1000.0 °C | 1.58E-5 - 1.7E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.58E-5 - 1.7E-5 1/K | |

Unlock all property charts | ||

Max service temperature, long | -196 - 450 °C Show Material materials with Max service temperature, long of -196 - 450 °C | |

Specific heat capacity | 20.0 °C | 410 - 415 J/(kg·K) Show Material materials with Specific heat capacity of 410 - 415 J/(kg·K) |

100.0 °C | 435 J/(kg·K) Show Material materials with Specific heat capacity of 435 J/(kg·K) | |

200.0 °C | 460 J/(kg·K) Show Material materials with Specific heat capacity of 460 J/(kg·K) | |

300.0 °C | 480 J/(kg·K) Show Material materials with Specific heat capacity of 480 J/(kg·K) | |

400.0 °C | 505 J/(kg·K) Show Material materials with Specific heat capacity of 505 J/(kg·K) | |

500.0 °C | 525 J/(kg·K) Show Material materials with Specific heat capacity of 525 J/(kg·K) | |

600.0 °C | 550 J/(kg·K) Show Material materials with Specific heat capacity of 550 J/(kg·K) | |

700.0 °C | 575 J/(kg·K) Show Material materials with Specific heat capacity of 575 J/(kg·K) | |

800.0 °C | 600 J/(kg·K) Show Material materials with Specific heat capacity of 600 J/(kg·K) | |

900.0 °C | 625 J/(kg·K) Show Material materials with Specific heat capacity of 625 J/(kg·K) | |

1000.0 °C | 650 J/(kg·K) Show Material materials with Specific heat capacity of 650 J/(kg·K) | |

Unlock all property charts | ||

Thermal conductivity | 20.0 °C | 9.8 - 10 W/(m·K) Show Material materials with Thermal conductivity of 9.8 - 10 W/(m·K) |

100.0 °C | 11.2 W/(m·K) Show Material materials with Thermal conductivity of 11.2 W/(m·K) | |

200.0 °C | 12.8 W/(m·K) Show Material materials with Thermal conductivity of 12.8 W/(m·K) | |

300.0 °C | 14.4 W/(m·K) Show Material materials with Thermal conductivity of 14.4 W/(m·K) | |

400.0 °C | 16.3 W/(m·K) Show Material materials with Thermal conductivity of 16.3 W/(m·K) | |

500.0 °C | 17 - 17.3 W/(m·K) Show Material materials with Thermal conductivity of 17 - 17.3 W/(m·K) | |

600.0 °C | 19.3 W/(m·K) Show Material materials with Thermal conductivity of 19.3 W/(m·K) | |

700.0 °C | 21 W/(m·K) Show Material materials with Thermal conductivity of 21 W/(m·K) | |

800.0 °C | 22.6 W/(m·K) Show Material materials with Thermal conductivity of 22.6 W/(m·K) | |

900.0 °C | 24.6 W/(m·K) Show Material materials with Thermal conductivity of 24.6 W/(m·K) | |

1000.0 °C | 26.7 W/(m·K) Show Material materials with Thermal conductivity of 26.7 W/(m·K) | |

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.28E-6 - 1.29E-6 Ω·m Show Material materials with Electrical resistivity of 1.28E-6 - 1.29E-6 Ω·m |

100.0 °C | 1.3E-6 Ω·m Show Material materials with Electrical resistivity of 1.3E-6 Ω·m | |

200.0 °C | 1.32E-6 Ω·m Show Material materials with Electrical resistivity of 1.32E-6 Ω·m | |

300.0 °C | 1.33E-6 Ω·m Show Material materials with Electrical resistivity of 1.33E-6 Ω·m | |

400.0 °C | 1.35E-6 Ω·m Show Material materials with Electrical resistivity of 1.35E-6 Ω·m | |

500.0 °C | 1.36E-6 Ω·m Show Material materials with Electrical resistivity of 1.36E-6 Ω·m | |

600.0 °C | 1.36E-6 Ω·m Show Material materials with Electrical resistivity of 1.36E-6 Ω·m | |

700.0 °C | 1.36E-6 Ω·m Show Material materials with Electrical resistivity of 1.36E-6 Ω·m | |

800.0 °C | 1.36E-6 Ω·m Show Material materials with Electrical resistivity of 1.36E-6 Ω·m | |

900.0 °C | 1.35E-6 Ω·m Show Material materials with Electrical resistivity of 1.35E-6 Ω·m | |

1000.0 °C | 1.32E-6 Ω·m Show Material materials with Electrical resistivity of 1.32E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.4 % Show Material materials with Aluminium of 0.4 % |

Carbon | 0.03 - 0.1 % Show Material materials with Carbon of 0.03 - 0.1 % |

Chromium | 20 - 23 % Show Material materials with Chromium of 20 - 23 % |

Cobalt | 1 % Show Material materials with Cobalt of 1 % |

Copper | 0.5 % Show Material materials with Copper of 0.5 % |

Iron | 5 % Show Material materials with Iron of 5 % |

Manganese | 0.5 % Show Material materials with Manganese of 0.5 % |

Molybdenum | 8 - 10 % Show Material materials with Molybdenum of 8 - 10 % |

Nickel | 55.45 - 58 % Show Material materials with Nickel of 55.45 - 58 % |

Phosphorus | 0.01 - 0.02 % Show Material materials with Phosphorus of 0.01 - 0.02 % |

Silicon | 0.4 - 0.5 % Show Material materials with Silicon of 0.4 - 0.5 % |

Sulfur | 0.01 - 0.015 % Show Material materials with Sulfur of 0.01 - 0.015 % |

Titanium | 0.4 % Show Material materials with Titanium of 0.4 % |